influence of commercial saturated monoglyceride, of commercial saturated monoglyceride, ......
Post on 22-Jun-2018
Embed Size (px)
Research ArticleInfluence of Commercial Saturated Monoglyceride,Mono-/Diglycerides Mixtures, Vegetable Oil, Stirring Speed, andTemperature on the Physical Properties of Organogels
Omar Gerardo Rocha-Amador,1 Jose Alberto Gallegos-Infante,1
Qingrong Huang,2 Nuria Elizabeth Rocha-Guzman,1
Martha Rocio Moreno-Jimenez,1 and Ruben F. Gonzalez-Laredo1
1 Unidad de Posgrado, Investigacion y Desarrollo Tecnologico, Departamento de Ings Qumica y Bioqumica,Instituto Tecnologico de Durango, Bulevar Felipe Pescador 1830 Ote., Colonia Nueva Vizcaya, 34080 Durango, DGO, Mexico
2Department of Food Science, School of Environmental and Biological Sciences, Rutgers University,The New Jersey State University, 65 Dudley Road, New Brunswick, NJ 08901, USA
Correspondence should be addressed to Jose Alberto Gallegos-Infante; email@example.com
Received 11 May 2014; Revised 25 July 2014; Accepted 16 August 2014; Published 21 September 2014
Academic Editor: Jose M. Prieto
Copyright 2014 Omar Gerardo Rocha-Amador et al. This is an open access article distributed under the Creative CommonsAttribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work isproperly cited.
The objective of this study was to evaluate the influence of gelator, vegetable oil, stirring speed, and temperature on thephysical properties of obtained organogels. They were prepared under varying independent conditions and applying a fractionalexperimental design. From there a rheological characterization was developed. The physical characterization also includedpolarized light microscopy and calorimetric analysis. Once these data were obtained, X-Ray diffraction was applied to selectedsamples and a microstructure lattice was confirmed. Commonly, the only conditions that affect crystallization have been analyzed(temperature, solvent, gelator, and cooling rate). We found that stirring speed is the most important parameter in the organogelpreparation.
Gels have been described as materials that are easier torecognize than define . Most of the times this problemcomes from industry, which develops products with a gelname, just to be attractive to consumers . However,gels have been accepted as semisolid materials comprisinglow concentrations (
2 International Journal of Food Science
Organogels microstructure is possible in part due to fatcrystallization. This phenomenon has been widely studied inseveral scientific fields. The case of fat oils is very importantdue to their applications in food industry. The study ofcrystal nucleation, dissolution, and agglomeration in theoverall precipitation scheme implies practical difficulties.Nucleation and crystal growth are spontaneous processes,which diminish the energy of the growing particle andnucleation process in order to overcome activation energy;that is, the critical cluster (critical size) is the cluster withmaximum Gibbs free energy. The activation barrier maybe represented by three parameters: supersaturation ratio,reaction temperature, and interfacial energy . Followingcrystal formation in organogels can give detailed informationon how their preparation is affecting their final structure.
The crystallization behavior is related to concentration ofgelator , cooling rate [11, 12], and shear rate on fat crystals[13, 14]. Depending on the system, gels are formed by differentforces and interactions and there are some parameters thataffect, such as pH, ionic force, and mechanical forces. Theplastic fat gels are formed due to the aggregation of fat crystalsby several forces as van der Waals, dipole-dipole, hydropho-bic, and hydrogen bond interactions between crystals .These interactions also give gels a fractal behavior. Fractal isa geometric pattern that is repeated at every smaller scale toproduce irregular shapes and surfaces .
Hence, since the study of organogels is very complex, itmust include structural analysis and rheological and thermalbehaviors in order to have a clear understanding on howpreparation parameters are affecting the final product. Thus,our objective was to evaluate the influence of gelator (typeand concentration), type of vegetable oil, stirring speed,and temperature preparation on the physical properties ofobtained organogels.
2. Materials and Methods
2.1.Materials. Three different vegetable oils (soybean, canola,and corn oil) were used. They have important differencesin composition of saturated fatty acids (SFA), monoun-saturated fatty acids (MUFA), and polyunsaturated fattyacids (PUFA). The approximate compositions of soybean(SFA 15.65%, MUFA 22.78%, and PUFA 57.74%, WessonBrand), canola (SFA 7.36%,MUFA63.27%, andPUFA28.14%,Wesson Brand), and corn (SFA 12.94%, MUFA 27.57%, andPUFA 54.67%, Mazola Brand) were considered. These oilswere bought at a local supermarket in New Brunswick(New Jersey,USA).Myverol (mainlymonoglycerides glycerylmonostearate 49%, glyceryl monopalmitate 48%, and cal-cium silicate 3%) and Myvatex (mixture of monoglyceridesand diglycerides, soy monoglycerides 3545%, stearic acidmonoester with propane-1-2-diol 4050%, sodium 2-stearoyllactate 1015%, and calcium silicate 3%) were provided byKerry, Mexico/USA, and used as gelator agents.
2.2. Gels Preparation. Gelators Myverol (MV) and Myvatex(MX) at three different concentrations (8, 9, and 10%) wereheated (70, 80, and 90C) on glass containers until completemelting, and then either vegetable oil (soy (SY), canola (CA),
or corn (CN)) was added. Samples were stirred (T 25 digitalUltra-turrax, IKA, North Carolina, USA) for five minutesat three independent speeds (3600, 7200, and 12000 rpm)to homogenize them; then, samples were cooled to roomtemperature and stored in refrigerator for 24 hours.
2.3. Rheological Tests. Dynamic frequency sweep tests wereperformed in a rheometer (ARES Rheometer 902-30004,TA instruments, New Castle, DE, USA) using parallel platesgeometry (25mm diameter) under the following experimen-tal settings: strain 0.1%, temperature 20C, frequency sweep0.1100 rad s1, and a gap of 1mm. The and modules,complex viscosity, and delta tangent for each experimentalsample were obtained.
2.4. Polarized Light Microscopy. Polarized light micropho-tographs of organogels were obtained using a polarizedlight microscope Linkam Brand (T95 System controller; T95Linksys 32 soft, 2009, Tadworth, UK). It was equipped witha Q imaging camera (Color RTV 10 BIT) using an OlympusTH4-100 Halogen lamp power supply unit (LTS120 temp.controlled stage). Images were taken at 20C, and video wastaken using the Camtasia Studio V 7.0 (Build 1426, 2010,Techsmith Corporation, Okemos, MN, USA).
2.5. Differential Scanning Calorimetry. Thermal behavior ofsamples was studied using a differential scanning calorime-ter (DSC Q2000 TA instruments, Schaumburg, Ill, USA)equipped with refrigerated cooling system (RCS 40 TAInstruments, Schaumburg, Ill, USA). Samples were heated at120C (30min) for deleting fat thermal memory. Up to threecycles of heating were used depending on the experimentalsample. Gelation temperature and melting enthalpy for eachexperimental sample were recorded.
2.6. X-Ray Diffraction. X-ray diffraction experiment wasdeveloped by the use of a PXRD conduced with a D/M-2200T automated system (Ultima Rigaku, Tokyo, Japan) withCu K radiation = 1.5406A. Patterns were collected at2 angles of 3 to 50 at a scan rate of 2/min. A graphitemonochromator was used and the generator power settingswere fixed at 40 kV and 40mA. Spectra were analyzed withspecialized software (Xpowder Pro Ver. 2010.01.30, Woburn,Massachusetts, USA) for clarifying peaks, applying a singlefunctional filter smoothing and five cycles of Fourier decon-volution.
2.7. Fractal Dimension. The fractal dimension of the sampleswas calculated using (1) according to a describedmethod ,which is based on the Avrami relationship. Consider
ln (1 cr) =
where cr is the crystallinity of the system; is time; is aconstant; and denotes the dimension of growing. and were calculated by nonlinear estimation using Levenberg-Marquardt algorithm (Statistica v 7.0, Tulsa, OK, USA). Crys-talline fraction of samples was calculated adjusting values
International Journal of Food Science 3
from complex viscosity of the system removing complexviscosity of the solvent:
2.8. Microstructural Parameters. A universal relation hasbeen developed , but in the present work a previousrelationship was used , supported by earlier theoreticalwork  in order to evaluate structural parameters. Inthis experimental work, a three-dimensional colloidal net-work was considered as being composed of interconnectedflocs and the fractal dimension was used to quantify therelationship between the average floc size and the particleconcentration of the colloidal network. The fractal natureof fat crystal networks has been already presented  andexplained the power-law relationship followed by andthe solid fat content (SFC) data for fat samples with lowsolid fat content (
4 International Journal of Food Science
Table 1: Gelation enthalpy comparison for organogel samples.
Process conditions g
Gelator (%) Stirring 1/min Temperature (C) Canola Corn SoyJ/g J/g J/g
Myverol 8 3600 70 5.90 (0.18) 4.87 (0.30) 5.80 (0.17)Myvatex 8 3600 90 5.72 (1.06) 4.54 (0.10) 2.38 (0.16)Myvatex 8 12000 70 4.94 (0.33) 5.96 (0.08) 5.57 (0.04)Myverol 8 12000 90 5.56 (0.06) 5.78 (0.46) 6.14 (0.26)Myvatex 9 7200 80 5.38 (0.48) 4.26 (0.18) 7.40 (0.20)Myverol 9 7200 80 7.04 (0.71) 6.52 (0.79) 6.83 (0.27)Myvatex 10 3600 70 6.61 (0.11) 5.60 (0.60) 6.66 (0.15)Myverol 10 3600 90 8.87 (0.25) 7.42 (0.30) 7.90 (0.45)Myverol 10 12000 70 7.50 (0.35) 7.31 (0.54